Available online at www.sciencedirect.com
Acta Materialia 60 (2012) 5160–5171
Hydrogen embrittlement of ferritic steels: Observations ondeformation microstructure, nanoscale dimples
and failure by nanovoiding
T. Neeraj a,⇑, R. Srinivasan b, Ju Li c,d
a ExxonMobil Development Company, Houston, TX 77060, USAb Corporate Strategic Research, ExxonMobil Research and Engineering, Annandale, NJ 08801, USA
c Department of Nuclear Science and Engineering, MIT, Cambridge, MA 02139, USAd Department of Materials Science and Engineering, MIT, Cambridge, MA 02139, USA
Received 12 March 2012; received in revised form 5 June 2012; accepted 6 June 2012Available online 24 July 2012
While hydrogen embrittlement of ferritic steels has been a subject of significant research, one of the major challenges in tacklinghydrogen embrittlement is that the mechanism of embrittlement is not fully resolved. This paper reports new observations and interpre-tation of fracture surface features and deformation microstructures underneath the fracture surface, providing a mechanistic view of fail-ure catalyzed by hydrogen. Linepipe grade ferritic steels were tested in air with electrochemically pre-charged hydrogen and in high-pressure H2 gas. The fracture surface features were studied and compared using high-resolution surface-sensitive scanning electronmicroscopy, and the deformation microstructures just beneath the fracture surfaces were studied using transmission electron microscopy.Significant dislocation plasticity was observed just beneath both ductile and quasi-brittle fracture surfaces. Further, the dislocation activ-ity just beneath the fracture surfaces was largely comparable with those observed in samples tested without hydrogen. Evidence forhydrogen-enhanced plastic flow localization and shear softening on the sub-micron scale was observed very near the final fracture surface(<2 lm) in the tensile samples. The quasi-brittle fracture surfaces were found to be covered with nanoscale dimples 5–20 nm wide and1–5 nm deep. Based on analyses of conjugate fracture surfaces, most of the nanodimples appear to be “valley-on-valley” type, rather than“mound-on-valley” type, indicating nanovoid nucleation and growth in the plastically flowing medium prior to ultimate failure. Based onthese observations, an alternative scenario of plasticity-generated, hydrogen-stabilized vacancy damage accumulation and nanovoidcoalescence as the failure pathway for hydrogen embrittlement is proposed.� 2012 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Keywords: Hydrogen embrittlement; Transmission electron microscopy; Fracture; Deformation structure; Ferritic steels
Hydrogen embrittlement of steels is a longstandingtechnological challenge in the oil and gas industry [1,2].Recently, hydrogen embrittlement of steels has been consid-ered one of the key challenges in storing and transportinghydrogen for the hydrogen economy . Therefore, it con-tinues to be an active area of research [4–7]. The current
1359-6454/$36.00 � 2012 Acta Materialia Inc. Published by Elsevier Ltd. All
⇑ Corresponding author.E-mail address: [email protected] (T. Neeraj).
understanding of the mechanism of hydrogen embrittle-ment is that hydrogen from the environment dissolves intosteel, migrates as atomic hydrogen towards internal stresscenters such as crack tips, and ultimately facilitates nucle-ation and propagation of cracks, leading to failure .While it is well accepted that hydrogen embrittlement iscaused by accumulation of atomic hydrogen at internal cen-ters of high triaxial stresses, the actual micromechanism offailure is not fully understood. Several groups have pro-posed different mechanisms for hydrogen embrittlement.The three major classes of the proposed mechanisms are
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5161
hydrogen-enhanced decohesion (HEDE) [9–11], hydrogen-enhanced localized plasticity (HELP) [12,13] and hydro-gen-enhanced vacancy stabilization mechanism (VM)[14,15]. In the HEDE mechanism, it is envisioned thathydrogen accumulation at locations of high triaxial stressesleads to weakening of Fe–Fe bonds beyond a critical hydro-gen concentration, leading to fracture [9,10]. This impliesthat any plasticity associated with hydrogen embrittlementis a consequence of the decohesion process and not thedirect cause of embrittlement. However, in a series of care-ful studies, Gerberich and co-workers showed that there isplastic deformation associated with hydrogen embrittle-ment [11,16]. Using super-dislocation models, Gerberichet al. proposed that dislocations emanating from crack tipsgreatly enhance local stresses a few nanometers ahead of thecrack tip to cause significant hydrogen accumulation (of theorder of 50 at.%), which leads to HEDE . The HELPmechanism is supported by in situ transmission electronspectroscopy (TEM) studies, where the introduction ofhydrogen gas has been shown to enhance dislocation mobil-ity in many metals and alloys. It was suggested that sliplocalization such as planar slip may be promoted in thepresence of hydrogen, leading to premature fracture. How-ever, the exact micromechanisms of the failure process werenot clearly identified in these studies [12,13]. Finally, in thecase of the VM model, the primary function of hydrogen inthe embrittlement process is envisioned to be the stabiliza-tion and promotion of vacancy agglomeration [14,15].There is indirect experimental evidence suggesting thatdeformation in the presence of hydrogen can lead to accu-mulation of excess vacancies in Fe and steel [17,18]. Thisaccumulation of excess vacancies is suggested to lower theductility in steels that fail through micro-void coalescence(MVC) [14,15]. Despite such a rich literature on boththeoretical and experimental work in this area, the actualmicromechanism of failure due to hydrogen embrittlementin ferritic steels is still not fully resolved. In the authors’view, there has been little systematic work comparing thedeformation microstructures from hydrogen embrittledfracture surfaces (both MVC fracture and quasi-brittle frac-ture features) with those from samples tested withouthydrogen. Further, there have been only a few studies onthe nanoscale characterization of the fracture surface fea-tures (topography).
Therefore, the primary goal of this work was to charac-terize the deformation microstructures associated withhydrogen-induced fracture as well as to characterize thefracture surface topography in high resolution to identifythe key micromechanisms that lead to hydrogen embrittle-ment. To this end TEM was employed to study deformationmicrostructures just underneath fracture surfaces, usingfocused ion beam (FIB) methods to extract TEM foils.High-resolution scanning electron microscopy (SEM) andatomic force microscopy (AFM) were used to study thenanoscale topographical features on hydrogen-embrittledquasi-brittle facets. Finally, the findings from this workare discussed in relation to prior literature and an
alternative nanovoid coalescence (NVC) micromechanismof hydrogen embrittlement for ferritic steels is proposed.
2. Experimental details
In the present work hydrogen embrittlement mecha-nisms were studied in linepipe grade steels by generatinghydrogen-embrittled fracture surfaces by testing in boththe hydrogen pre-charged condition and in high-pressurehydrogen gas.
2.1. Materials and hydrogen pre-charged testing
In one set of studies, X65 (yield strength (YS) 448 MPa)and X80 (YS 550 MPa) grade steels were electrochemicallypre-charged with 4 wt.ppm of total hydrogen and 1 wt.ppmof diffusible hydrogen using a solution of 5 mg l�1 As2O3
and 0.5 M H2SO4, at a current density of 5 mA cm�2 for4 h. The total hydrogen content was measured with a Lecoanalyzer. The diffusible hydrogen content was measuredusing thermal desorption spectroscopy analysis, where allthe hydrogen that was evolved up to 300 �C was designatedas diffusible hydrogen . Tensile tests on electrochemi-cally pre-charged X65 and X80 steel samples were con-ducted at a strain rate of 10�5 s�1 immediately after pre-charging. For the same set of steels, single-edge notchedbend (SENB) tests were conducted immediately after elec-trochemical pre-charging at a K rate of 0.03 MPa
2.2. Materials and testing in gaseous hydrogen
A second set of fracture toughness tests were conductedusing compact-tension specimens on X52 (YS 358 MPa),X60 (YS 413 MPa) and X80 (YS 552 MPa) grade linepipesteels in high-pressure H2 gas under pressures of 5.5 MPa,21 MPa and 103 MPa. These tests were conducted at San-dia National Laboratories, and tested coupons were pro-vided for this study. Details of this testing and themechanical properties for these samples are reported else-where [20,21].
The foils for TEM studies were prepared by both stan-dard electropolishing and FIB lift-out techniques usingFEI-Helios dual-beam FIB. Electropolishing was per-formed in a Fischione Model 110 twin-jet electropolishingunit, using a solution of 30 ml perchloric acid (70%),300 ml methanol and 175 ml butyl alcohol at a temperatureof �40 �C. In the FIB lift-out from fracture surfaces, carewas taken to prepare foils with the fracture surface pre-served (through Pt deposition on the surface) so that onecould make deformation microstructure observations fromjust beneath the fracture surface to several micrometersaway from the fracture surface. In the results reported inthis work, the thin end of the foil represents the fracturesurface. Samples were also prepared for microstructure
5162 T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171
analysis of as-received materials using the electropolishingprocedure described above and using FIB lift-out. TEMstudies were conducted in a Philips CM200 microscopeoperating at an accelerating voltage of 200 kV. The micro-structure analyses were performed using both conventionaldiffraction contrast techniques and bright-field scanningtransmission electron microscopy (BF-STEM) mode. Con-ventional fractography was performed by SEM in a JEOL6460-LV microscope with a LaB6 cathode operated at15 kV. High-resolution SEM analysis of fracture surfacefeatures was performed in a LEO-1530 field emission gun(FEG) at an operating voltage of 3–7 kV with a shortworking distance of 3–5 mm. AFM observations were per-formed using an Asylum Research Cypher microscope.
3.1. As-received microstructure
The as-received microstructure of the H pre-chargedsamples is shown in Fig. 1. The X65 linepipe steel had adual phase ferritic–pearlitic microstructure. The ferritephase had a grain size of �10 lm, with a sub-grain sizeof 1–3 lm (developed during the thermo-mechanical pro-cessing of the linepipe). The X80 steel had a ferritic–bainit-ic microstructure and had ferrite grain size and sub-grainsizes nominally similar to the X65 steel. The as-receivedsub-grain structure was observed to be the same in TEMfoils prepared by both electropolishing and FIB extraction.
Fig. 1. (a, b) As-received microstructure of X-65 steel used in pre-chargemicrostructure of X-80 steel used in pre-charged H studies showing ferrite–ba
The microstructure of samples tested in high-pressurehydrogen gas ranged from ferrite–pearlite to acicular fer-rite, depending on the grade of steel, and was previouslyreported by San Marchi et al. [20,21].
3.2. Fractography and deformation microstructure ofhydrogen pre-charged samples
3.2.1. Tensile tested specimens
Tensile tests of electrochemically H pre-charged X65steel exhibited a decrease in ductility from 15% failurestrain for the uncharged condition to 12% failure strainafter H pre-charging. Examination of the fracture surfacesby SEM showed that, in both cases, fracture occurred byMVC. There was no apparent change in the failure modeafter H pre-charging. In the case of X80 steel, the failurestrain was 10% in the uncharged condition and decreasedto 8% in the H pre-charged condition. However, in the Hpre-charged X80, the fracture mode was significantlyaltered compared with the uncharged condition. As shownin Fig. 2a, the uncharged X80 steel failed by MVC. How-ever, the H pre-charged X80 exhibited a mixed mode offracture showing both MVC (on the outside) and quasi-brittle fracture at center of the sample (see Fig. 2b).
Thin foils were then extracted from the fracture surfaceof tensile coupons using FIB methods to analyze the defor-mation microstructure associated with the fracture. In thecase of X65, the deformation microstructure underneaththe MVC fracture regions from both the uncharged and
d H studies showing ferrite–pearlite microstructure. (c, d) As-receivedinite microstructure.
Fig. 2. (a) MVC or ductile fracture observed in uncharged X80 tensile sample. (b) Quasi-brittle fracture observed in H pre-charged X80 tensile sample.
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5163
H pre-charged specimens were analyzed. In the case of X80tensile specimens, observations of deformation microstruc-ture from both MVC fracture regions (both uncharged andH pre-charged condition) and the quasi-brittle fractureregions (in H pre-charged condition) were performed.These results are discussed next.
In Fig. 3a and b, the deformation microstructurebeneath the fracture surface of an uncharged X65 MVCfracture is presented. The edge of the foil is the fracture sur-face and is towards the top in all the micrographs presentedin this paper. Thus, these micrographs constitute observa-tions that extend right from the fracture surface to severalmicrometers below the fracture surface. Key observationsfrom Fig. 3a and b include (a) a very high dislocation den-sity below the fracture surface, indicative of extensive plas-ticity, and (b) a highly refined sub-grain structure with sub-grain sizes of �150–300 nm, compared with the startingsizes of 1–3 lm. In some regions, one can observe a seriesof microvoids of varying sizes nucleating and growing atthe sub-grain boundaries (e.g., see Fig. 3b).
The deformation microstructure from H pre-chargedX65 is shown in Fig. 3c–e. Again a very high dislocationdensity and refined sub-grain structure were observed.While the overall deformation microstructure immediatelybeneath the fracture surface was similar to the unchargedX65, one key difference in the case of the H pre-chargedX65 was the observation of dramatic gradation in the
0.5 µµm 0.5 µm
(a) (b) (c)
Fig. 3. (a) Deformation microstructure underneath MVC fracture surface shArrows indicate nucleation of microvoids at sub-grain boundaries in unchargindicating strong gradation in sub-grain structure (indicated by arrow). (d) Higgrain structure observed underneath the fracture surface. (e) Deformation mincrease in sub-grain size. Note: in all the micrographs, the fracture surface is
sub-grain structure. Superfine sub-grain structures (�50–100 nm) were observed 1–2 lm from the fracture surface(see Fig. 3c and d) which transitioned to coarser (200–300 nm) sub-grains >3 lm away from the fracture surface(Fig. 3e). The significance of these observations is discussedlater.
The deformation microstructure from MVC regions ofuncharged X80 steel indicated high dislocation densityand refined sub-grain structure consistent with the observa-tions made in uncharged X65 steel. The deformationmicrostructure from a quasi-brittle facet in H pre-chargedX80 steel is shown in Fig. 4a and b. Interestingly, thisregion also showed extensive dislocation plasticity, accom-panied by refinement of the sub-grain structure. More sig-nificantly, there was a gradation in sub-grain size (indicatedby an arrow in Fig. 4a), with very fine sub-grain structureat the fracture surface and coarsening of the structure awayfrom the fracture surface. Fig. 4c and d shows the deforma-tion microstructure beneath a ductile (MVC) fractureregion from the same specimen. Again, there was refine-ment of the sub-grain structure and significant dislocationdensity indicative of extensive plasticity. Further compari-son of the deformation microstructure between MVC(Fig. 4c and d) and quasi-brittle regions (Fig. 4a and b)in H pre-charged X80 steel indicated that they were indis-tinguishable. To reiterate, the deformation microstructureunderneath the fracture surface of both the MVC region
100 nm 200 nm
owing refined sub-grain structure in uncharged X65 tensile sample. (b)ed X65 tensile sample. (c) Microstructure in H pre-charged X65 tensile,
her magnification of the marked area in Fig. 3c, showing the very fine sub-icrostructure from an area �1 mm away from fracture surface, showingtowards the top of the picture.
500 nm 500 nm
500 nm 100 nm
(a) (b) (d)(c)Quasi- Ductile
Fig. 4. (a, b) Deformation microstructure underneath quasi-brittle fracture facet in H pre-charged X80 tensile sample showing significant dislocationplasticity leading to refined sub-grain structure. Arrow in Fig. 4a indicates gradation in sub-grain structure, with very fine sub-grains near the fracturesurface. (c) Deformation microstructure underneath ductile fracture (MVC) feature in H pre-charged X80 tensile sample. Dislocation plasticity leading torefined sub-grain structure is evident. (d) Dislocation substructure within a sub-grain beneath ductile fracture feature, showing high dislocation density,indicative of significant plasticity.
5164 T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171
and the quasi-brittle facet in H pre-charged X80 steel werequite similar and consistent with those observed in H pre-charged X65 steel. This further suggests that, in the pres-ence of hydrogen, significant dislocation plasticity is associ-ated with not only ductile fracture, but also quasi-brittlefracture.
3.2.2. SENB tested specimens
Fractography of uncharged X80 steel in SENB testingshowed MVC fracture, while the H pre-charged sampleshowed quasi-brittle fracture with no evidence of MVCfracture (Fig. 5a). The dislocation structure underneaththe fracture surface was studied in both uncharged X80and H pre-charged X80 steel. In the uncharged X80, therewas significant dislocation plasticity with a high dislocationdensity in a 1–2 lm zone directly beneath the fracture sur-face, but the as-received sub-grain structure was preserved.As shown in Fig. 5b and c, the deformation microstructurein H pre-charged X80 also exhibited significant plasticityand high dislocation density, with no significant changein the sub-grain structure. Comparing the two conditions,even though the fracture mode changed from MVC toquasi-brittle fracture due to H pre-charging, the underlyingdeformation microstructure (up to a few micrometers
Fig. 5. (a) Quasi-brittle fracture observed in H pre-charged X80 SENB samindicating significant dislocation plasticity in H pre-charged X80 SENB samp
below the fracture surface) remained quite similar andcomparable. Studies comparing the uncharged and Hpre-charged X65 steel in SENB testing were also con-ducted, and these results were quite similar and consistentwith observations presented for X80 steel above. Finally, itshould be noted that the key difference in the deformationmicrostructure between the tensile and SENB samples wasthe lack of refined sub-grain structure in the SENBsamples.
3.3. Fractography and deformation microstructure ofspecimens tested in hydrogen gas
When the samples were tested under high-pressure H2
gas (instead of electrochemically pre-charging with H),conventional fractography indicated that quasi-brittle frac-ture occurred at all hydrogen gas pressures and in all threegrades (X52, X60 and X80) of steels tested. TEM foils wereextracted from quasi-brittle facets from X60 samples testedin hydrogen gas pressures of 5.5 MPa, 21 MPa and103 MPa, respectively. Examples of deformation micro-structure underneath the quasi-brittle fracture facets fromX60 tested at 5.5 MPa and 103 MPa H2 gas pressures areshown in Fig. 6. All three samples showed high dislocation
ple. (b, c) Deformation microstructure underneath quasi-brittle facets,le.
200 nm 50 nm200 nm 50 nm
5.5 MPa 103 MPa(a) (b) (d)(c)
Fig. 6. Deformation microstructure underneath quasi-brittle facets indicating significant dislocation plasticity in X60 CT samples tested in high-pressurehydrogen gas at (a, b) 5.5 MPa and (c, d) 103 MPa.
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5165
densities and significant plasticity, with no significantreduction in the sub-grain sizes from the as-received mate-rial. There were no apparent differences in the deformationmicrostructure among the three samples. These results areconsistent with the deformation microstructures observedin H pre-charged X65 and X80 steels.
3.4. High-resolution SEM of quasi-brittle fracture facets
The deformation microstructure observations presentedabove show that there was significant plasticity occurringduring hydrogen-induced fracture, whether tested withpre-charged hydrogen or in high-pressure H2 gas. How-ever, conventional fractography studies indicated quasi-brittle fracture, and there was no apparent evidence yetfor manifestation of this plasticity on the fracture surfacetopography. Further, in the case of X80 tensile studies withpre-charged hydrogen, the deformation microstructure wasindistinguishable between a MVC fracture region and aquasi-brittle fracture region immediately beneath the frac-ture surface. In order to further explore evidence for man-ifestation of the underlying plasticity, advanced SEMfractography was performed, using imaging conditionsmore surface sensitive than conventional imaging condi-tions (see Section 2.3 for details).
Examples of typical quasi-brittle fracture features inhydrogen pre-charged X65 and X80 steels tested in SENBimaged in surface-sensitive imaging conditions are shownin Fig. 7. At low magnifications, the fracture featuresappear as quasi-brittle facets typically reported in the
10µµm 200nm 1
Fig. 7. (a) Typical quasi-brittle fracture observed in H pre-charged X65 SENBfracture surface shows “mottled” contrast, indicating the presence of nanoscabrittle fracture observed in H pre-charged X80 SENB sample. (b) Higher ma“mottled” contrast similar to X65 SENB samples.
literature. However, when the quasi-brittle features areimaged at high magnifications, one can observe that thefracture surface exhibits a “mottled” contrast, with dark–bright contrast on the nanometer-scale. Upon close exam-ination, it is apparent that the mottled contrast is due todense coverage of “nanodimple”-like features on the frac-ture surface. It is interesting to note that these nanodimplescover the whole fracture surface in samples that fail byquasi-brittle fracture. Further, such nanodimples were alsoobserved on quasi-brittle facets of the pre-charged X80steel in tensile testing.
High-resolution imaging of quasi-brittle facets was per-formed on all the samples tested in high-pressure H2 gas.Again it was observed that the nanodimples were ubiqui-tous on the fracture surface in all the grades of steel tested(X52, X60 and X80) and for all hydrogen gas pressures. Atypical example from X80 steel tested in H2 gas at a pres-sure of 21 MPa is shown in Fig. 8.
In order to obtain further evidence that the mottledcontrast was produced by features that are due to nano-dimples, observations were performed on the same quasi-brittle facet on both halves of the conjugate fracturesurfaces. Such analysis of the nanodimple features was con-ducted on several samples. In Fig. 9, typical examples ofconjugate surface analysis from pre-charged X65 steeltested in SENB and from the X80 steel tested in 21 MPahydrogen gas pressure are shown. Examples of clusters ofthe same nanodimple features on both halves are circledin Fig. 9. One can observe that these features are not mat-ing pairs with a ligament on one half and dimple on the
sample. (b) Higher magnification view of a small region in Fig. 7a. Thele dimples on hydrogen-embrittled quasi-brittle facets. (c) Typical quasi-gnification view of a small region in Fig. 7c. The fracture surface shows
Fig. 10. AFM topography image from a quasi-brittle facet in H pre-charged X65 SENB sample showing the topography from thenanodimples.
Fig. 8. (a) Typical quasi-brittle fracture observed in X60 CT sample tested in 21 MPa hydrogen gas pressure. (b) Higher magnification view of a smallregion in Fig. 8a. The fracture surface shows “mottled” contrast, indicating the presence of nanoscale dimples on hydrogen-embrittled quasi-brittle facets.This is similar to the observations in H pre-charged SENB samples.
(a) (b) (c)
Fig. 9. (a, b) Conjugate surfaces of a quasi-brittle facet in H pre-charged X65 SENB sample. (c, d) Conjugate surfaces of a quasi-brittle facet in X80 CTsample tested under 21 MPa high-pressure hydrogen gas. Both sets of micrographs show that the “mottled” contrast is from nanodimples on quasi-brittlefacets. Some of the larger nanodimples or a cluster of nanodimples have been identified by circles/ovals on both halves, showing that they are indeednanovoids. A few features which represent mating features on conjugate surfaces have been marked with squares. See text for details.
5166 T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171
other half. In other words, they appear to be nanodimpleson both halves of the conjugate surfaces, and hence are twohalves of a nanovoid on the fracture surface. Contrastingthis are a few features that were marked with rectangleson both sets of fracture surfaces. These features are matingon the two halves; in other words, what is a void on onehalf of the sample is a ligament on the other half of thesample. Here, it should be noted that conjugate surfaceobservations of these features are very challenging for acouple of reasons. First, these features are on the nanome-ter-scale (typically of order 10–20 nm). This makes it quitechallenging to identify and locate the same features on con-jugate halves of the fracture surface. More importantly, thetwo halves of the fracture surface can never be mounted inexactly the same orientation for imaging, owing to samplemisalignment as well as to the fracture topography itself.For example, in one half of the sample, a feature can beoriented towards the detector and can be imaged well,while in the other half the same feature can be inclinedor could be shadowed owing to the fracture surface topog-raphy and cannot be imaged under exactly the same orien-tation and imaging conditions. Taking into considerationthese challenges, Fig. 9 still shows that the majority of dim-ple-like features on the fracture surface would indeed beconsistent with nanovoids.
In addition to the SEM studies, limited AFM studieswere performed on the pre-charged X65 steel tested inSENB to characterize the surface topography. As shownin Fig. 10, the nanodimple-like features are apparent from
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5167
the topographical image. Based on preliminary image anal-ysis the nanodimple features ranged in size from 5 to20 nm; however, they appear to be relatively shallow, witha depth of 1–5 nm. In summary, it appears that the plastic-ity associated with hydrogen embrittlement in ferritic steelsmanifests itself as nanodimple like features on the fracturesurface.
In this work, for the first time, comprehensive analysisof the deformation microstructure in hydrogen-embrittledsamples was performed, comparing different strengthgrades, pre-charged hydrogen vs testing in high-pressureH2 gas, and tensile tests with fracture toughness tests. Inthis section, these results are discussed in the context ofthe literature. Further, based on the results of this work,an alternative micromechanism for hydrogen embrittle-ment in ferritic steels is proposed in the next section.
One of the key observations across the board on all thesamples was that there was significant dislocation plasticityimmediately beneath the fracture surface in the presence ofH, even in samples that show quasi-brittle fracture. Asshown in Figs. 3 and 4, the deformation microstructurein the tensile samples indicated very high dislocation den-sity with refinement of the initial sub-grain structure. Theauthors are not aware of any work in the literature wherethe deformation microstructures underneath fracture sur-faces from tensile tests have been systematically studiedwith and without hydrogen pre-charging. Strong changesin sub-grain structure are an indication of significant plas-ticity due to accommodation of shape change of grains dur-ing deformation. Observations of refinement of the sub-grain structure have been made in deformation microstruc-ture analysis of rolled metals as well as in situ deformationstudies by TEM [22–24]. The observed reduction in sub-grain size starting at 1–3 lm to <300 nm is a clear indica-tion that significant plastic deformation had occurredbefore final failure in the tensile testing. Further, the factthat this change in sub-grain structure was similar in sam-ples with and without pre-charged hydrogen is an indica-tion that similar deformation processes are operative inboth sets of samples. However, one key difference was that,in the pre-charged samples, there was evidence for plasticflow localization very near the final fracture surface(1–2 lm) in both X65 and X80 steels. In the case of thepre-charged X65, one may argue that the conventionalnecking of ligaments between micro-voids can lead to thesuperfine sub-grain structure near the final fracture surface.But such a strong gradation in sub-grain structure was notobserved in the uncharged X65 sample that also failed byMVC fracture. Also, evidence for plastic flow localizationwas observed underneath a quasi-brittle fracture facet inthe pre-charged X80. Taking into consideration all theseobservations, it can be stated that there was evidence forhydrogen-enhanced plastic flow localization in the pre-charged tensile samples in the sense that the introduction
of pre-charged H must have shear-softened the materialon the length scale of several hundred nanometers to afew micrometers close to the eventual fracture plane. Whilethese observations are consistent with proposals of HELPtheory [12,13], it is worth noting that there was no directevidence for slip planarity. Further, the exact microscopiccause(s) for this shear-softening length scale cannot bedetermined by the current experiments and must await fur-ther experimentation and modeling .
In the pre-charged SENB samples, both X65 and X80failed by quasi-brittle fracture. In both cases, there was sig-nificant dislocation plasticity, but no apparent evidence forrefinement of sub-grain structure. The deformation micro-structure of X60 CT samples tested in hydrogen gas atthree different gas pressures also showed significantcrack-tip plasticity. While there was a qualitative reductionin dislocation density away from the fracture surface in allthe fracture toughness samples (both pre-charged andhydrogen gas tested samples), there was no clear evidencefor any dramatic gradation in plasticity away from the finalfracture surface comparable with the pre-charged tensilesamples. While there is little literature available to comparethe deformation microstructure observations from hydro-gen pre-charged samples, the dislocation structuresobserved in the high-pressure hydrogen gas tested samplescan be compared with those reported recently by Martinet al. [6,7] on a similar linepipe grade steel tested underhigh-pressure H2 gas. They also reported significant dislo-cation plasticity and dense dislocation networks under-neath hydrogen-induced quasi-brittle fracture features.While there is no comment on this aspect, based on thepublished micrographs there was no apparent reductionin sub-grain size close to the fracture surface in their studieseither. This means that, if hydrogen-enhanced plastic flowlocalization and shear softening preceded the eventualfailure for these cases, it did not lead to refinement ofsub-grain structure. This could be due to the following rea-sons: for the tensile samples, the shear-softening lengthscale, damage pattern gradation and the eventual fractureplane are self-evolved from an initially macroscopicallyuniformly deforming sample that exhibits significant dislo-cation plasticity. But for the SENB samples, the introduc-tion of an external notch restricted the plasticity to nearcrack-tip regions, and the amount of plasticity is reducedcompared with a tensile sample owing to high stress triax-iality. Therefore, the effects of hydrogen-enhanced plasticflow localization and shear softening could be subtle inthe SENB samples, and additional work is needed to estab-lish the length scale.
As discussed in Section 3.4, the quasi-brittle fracturesurfaces were characterized at high resolution by SEMfor indications of the significant plasticity observed in theTEM studies on the fracture surface. As shown in Figs.7–10, the most dramatic observation of the hydrogenembrittled quasi-brittle facets was the dense coverage ofnanodimples as the final imprint of the fracture process.These nanodimples have been observed in pre-charged
Fig. 11. Micrograph of a brittle facet in X80 generated by fracturing inliquid nitrogen (LN2). The fracture surface was imaged under conditionssimilar to those used to reveal the nanodimple structure in hydrogenembrittled quasi-brittle facets. It is clear that the “mottled” contrast andthe nanodimples are absent in the LN2-generated quasi-brittle facet.
5168 T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171
X80 tensile samples that had quasi-brittle facets as well asall the fracture toughness samples for all strength gradesexamined with either pre-charged hydrogen or those testedin hydrogen gas. Further, as shown in Fig. 9 these nano-dimples are apparently due to nanovoids on the fracturesurface. The most recent work by Martin et al.  reportedsimilar nanodimple-like features being observed in linepipegrade steel tested in high-pressure H2 gas. However, theyhave characterized these features as mounds and valleysthat occur after the final separation as a result of the relax-ation processes associated with the underlying dislocationstructure.
Conventional MVC fracture can be thought of as “hole-joining fracture” . There are four main steps in the for-mation of MVC fracture with this perspective. They are (i)nucleation of voids, (ii) growth and coalescence of voids toform a crack, (iii) extension of the crack by further nucle-ation and growth of voids ahead of the crack tip and (iv)final separation of the outer rim by shearing . Afterthe final fracture of a MVC process described above, thefracture surface contains dimples as the final signature ofthe ductile fracture that led to the failure. Analogous tothe microvoids/dimples as a signature of “hole-joining frac-ture” (i.e., a typical ductile fracture) on the micrometer-scale, the nanodimples observed on the quasi-brittle facetsof hydrogen embrittled samples can be interpreted as a sig-nature of “hole-joining fracture” at the nanometer-scale.Typically, during MVC fracture in steels, the nucleationof the voids occurs due to interface decohesion or crackingof inclusions or carbides or other hard second-phase parti-cles that are of the order of micrometers in size. Thesevoids will be separated by relatively large distances (severaltens or hundreds of micrometers), depending on the micro-structure of the material. Hence, for a NVC fracture pro-cess, the nanodimple nuclei must be very small. Further,they may need to be very high in density and need to belocalized near the eventual fracture surface to be consistentwith the experimental observations.
In the last decade Nagumo and co-workers proposed theso-called vacancy model (VM) where it is suggested thatthe primary function of hydrogen in hydrogen embrittle-ment is the stabilization and promotion of vacancyagglomeration [14,15]. Sakaki et al. performed positronannihilation studies and provided evidence for excessvacancy accumulation during deformation in the presenceof hydrogen . Takai et al.  performed a series ofinterrupted tensile tests in iron and IN625 with hydrogenpre-charging and provided evidence that the “damage” cre-ated during deformation in the presence of hydrogen per-sists even when the diffusible hydrogen is allowed toevolve out of the sample. They attribute this to excessvacancy accumulation during deformation in the presenceof hydrogen . However, owing to a lack of microscopyobservations, it is unclear how the accumulation of excessvacancies manifests itself in the deformation microstruc-ture and on the fracture surface. Further, Nagumo andco-workers have not proposed a micro-mechanism by
which vacancy accumulation can lead to macroscopic frac-ture (including quasi-brittle fracture).
In the literature, there is extensive discussion on thevacancy mechanism for void nucleation in the areas of duc-tile fracture in pure metals and radiation-damaged materi-als [24,27–31]. Cuitino and Ortiz  modeled nucleationof voids in pure face-centered cubic metals and suggestedthat such voids can indeed nucleate and grow to a criticalsize during quasi-static testing timescales by a diffusive pro-cess. They also suggested that these voids could grow byconventional plasticity once they grow to a critical sizedetermined by the inter-dislocation distance (estimated tobe 10–30 nm in highly deformed regions). Zinkle et al. performed elasticity calculations on the stability ofthe vacancy clusters to form voids. Their calculations indi-cated that the very small voids can only be stable in thepresence of gaseous impurities such as O, H and He. Morerecently, Bringa and co-workers [32–34] published a seriesof papers on the atomistic mechanism of void growthand suggested that even very small voids (e.g., 2–3 nm)can grow purely by dislocation processes without the needfor diffusive processes (if the applied stress is high enough).However, the calculations assume an initial void size of 2–3 nm that has already been nucleated, therefore, do notdirectly the address the void nucleation process. Based onthe available information discussed above, one can reason-ably expect that nanovoids can nucleate and grow in thepresence of excess vacancies.
Fig. 11 shows a brittle fracture facet from a pre-chargedX80 SENB sample that was fractured in liquid nitrogenand imaged under similar conditions. In comparison withFigs. 7–9, it is apparent that the nanodimple-like featuresare absent in the brittle fracture facet produced by fractur-ing in liquid nitrogen. This indicates that temperature mayplay a significant role in the generation of nanodimplefeatures, and therefore it is likely that coupled diffusive–
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5169
displacive processes play a role in the nanovoid nucleationand growth [35,36].
5. NVC micromechanism of hydrogen embrittlement
Based on the observations from this work, an alternativenanovoid nucleation, growth and coalescence micromecha-nism for hydrogen embrittlement is proposed below andshown schematically in Fig. 12a and b. This mechanismis developed from the point of view that contributions tomaterial toughness from dislocation plasticity are reducedor short-circuited in the presence of hydrogen. This occursin four stages and leads to fracture with reduction in tough-ness (or ductility). It is envisioned that initially upon load-ing in Stage I, the material deforms ahead of the crack tipand starts generating dislocation plasticity. Based on con-tinuum analysis, this plastic zone is initially on the orderof 1 mm for a material with a yield strength of 500 MPaand a fracture toughness of 50 MPa m1/2 . However,in the presence of hydrogen (either from pre-charging orfrom high-pressure H2 gas), hydrogen accumulates inregions of high hydrostatic stresses (e.g., near the cracktip). Furthermore, this hydrogen accumulation can beaccentuated by dislocation-assisted convection, as pro-posed by the HELP mechanism [12,13]. The accumulationof H leads to localization of plasticity within the plasticzone in regions with high local hydrogen content. It leadsto Stage II, where intense plasticity occurs in the regionswith higher hydrogen concentrations very near the cracktip. This region of localized deformation is designated asthe HELP zone and is consistent with HELP theory
Stage II Stage III
Nano-void Coalescence Mechanism
• Localized plasticity • Hydrogen accumulation • HELP Zone
• Excess Vacancy Accumulation
• Hydrogen-Vacancy Complexes
• Vacancy induced NaVoid nucleation and growth
Fig. 12. Schematic of NVC mec
[12,13]. Based on the TEM observations, this localizationof plasticity does not necessarily produce slip bands or pla-nar slip, but rather intense plastic flow localization on themesoscale. In the case of tensile testing, this plastic flowlocalization zone is <1 lm, while in the fracture toughnesstesting it is apparently several micrometers in diameter. It iswell known that dislocation plasticity generates excessvacancies [24,27,28,38]. The experimental work of Nagumoand co-workers [17,18] and other first-principles calcula-tions [39,40] have shown that hydrogen binds strongly withvacancies in body-centered cubic Fe. Therefore, in StageIII it is proposed that in the HELP zone next to the cracktip, there is generation and accumulation of excess vacan-cies that is stabilized by hydrogen binding to the vacancies.A tipping point is reached, through attainment of a criticallocal excess vacancy concentration that leads to Stage IV,where nucleation and growth of nanovoids occurs, leadingto ultimate failure (fracture) by nanovoid coalescence. Sucha mechanism can explain the quasi-brittle fracture surfacedensely covered with nanodimples (typically 5–20 nm). Itis also consistent with the previous hydrogen embrittlementtheories in that there is a need for critical hydrogen accu-mulation in a local volume to initiate the failure process,as has been proposed by the HEDE mechanism [9–11].The resulting plastic flow localization is consistent withthe HELP mechanism. Finally, the proposed mechanismprovides a micromechanical pathway for failure consistentwith the VM proposed by Nagumo [14,15]. Thus, the NVCmechanism implies that, while previously proposed models(HEDE, HELP and VM) can all be operative in the hydro-gen-embrittlement process, no single mechanism can
Stage II Stage III Mechanism Proposed by Martin et al
• Hydrogen accumulation • Localized plasticity • Weakened HELP Zone
• Decohesion • Surface relaxtion • Nanoscale mounds and
valleys • Mating fracture surfaces
hanism. See text for details.
5170 T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171
completely explain all the associated microstructural fea-tures. Rather, the NVC mechanism suggests that a combi-nation of elements of the previously proposed mechanismsis essential for rationalization of the microstructuralobservations.
Finally, Martin et al.  suggested that the evolveddeformation microstructure and local hydrogen concentra-tion establish weak regions, which dictate the local crackpath and the topology of the fracture surface. This is con-sistent with the micromechanical processes proposed in thiswork. However, Martin et al. suggest that the observednanodimple structure is associated with relaxation pro-cesses that occur after final decohesion or separation. Asillustrated in Fig. 12c, this would suggest that the conjugatefracture surfaces will be mating surfaces, where a dimple onone face will be a ligament or mound on the opposing face.While there is evidence for such features on the fracturesurface, the majority of the features appear to be valleyson both conjugate surfaces (see Fig. 9).
In summary, the proposed plasticity-generated, hydro-gen stabilized vacancy damage, vacancy aggregation andNVC mechanism provides a more complete mechanisticand microstructure-based explanation of hydrogen embrit-tlement in ferritic steels. The exact atomistic processes asso-ciated with nanovoid nucleation and growth in hydrogencharged steels needs further investigation. This is currentlybeing pursued by the authors, using atomistic methods,and will be published separately .
In this work, deformation microstructure and disloca-tion structure beneath quasi-brittle and MVC regions offracture surfaces generated in the presence and absence ofhydrogen were studied using FIB/TEM methods. Further,the fracture surface topography was studied on the nano-meter scale, using FEG-SEM under surface-sensitive imag-ing conditions and using AFM. Specifically, the followingconclusions are drawn from this work.
1. Significant dislocation plasticity has been observed to beassociated with hydrogen-embrittlement of ferriticsteels. Specifically, there was evidence of sub-grain struc-ture refinement underneath MVC regions and dense dis-location networks underneath quasi-brittle facets inlinepipe grade ferritic steels fractured under a varietyof testing conditions. These include tensile and fracturetoughness testing with either pre-charged hydrogen or inhigh-pressure H2 gas.
2. There was evidence for hydrogen-enhanced plastic flowlocalization at the mesoscale in the presence of hydro-gen, especially in tensile tested samples.
3. High-resolution SEM studies of conjugate fracture sur-faces of quasi-brittle facets provide evidence for fracturedue to nanovoids in the presence of hydrogen. Thismanifests as nanoscale (10–20 nm) dimples on the frac-ture surface.
4. By means of fracture surface and microstructural obser-vations, an alternative micromechanism based on plas-ticity-generated, hydrogen-stabilized vacancy damageand vacancy-induced nanovoid nucleation and coales-cence (NVC) is proposed as the failure mechanism lead-ing to quasi-brittle fracture in the presence of hydrogenin ferritic steels.
The authors acknowledge the help of Dr RamgopalThodla of DNV for performing the electrochemical pre-charging and mechanical testing of the X65 and X80 sam-ples. They also appreciate and acknowledge the tremen-dous help of Dan Huber of The Ohio State University inpreparing the FIB foils from the difficult fracture surfaces.T.N. would like to thank Dr Brian Somerday at SandiaNational Laboratories, Livermore, CA, for providing thehigh-pressure H2 gas tested specimens. J.L. would like toacknowledge financial support by ExxonMobil Researchand Engineering and partial support by NSF CMMI-0728069. Finally, the authors would like to thank Dr DaliaYablon of Corporate Strategic Research, ExxonMobil Re-search and Engineering for performing the AFM studies.
 Merrick RD. Mater Perform 1989;28:53–5. Rhodes PR, Skogsberg LA, Tuttle RN. Corrosion 2007;63:63–100. Somerday BP, Sofronis P, Jones R. Effects of hydrogen in materi-
als. Jackson Hole (WY): ASM International; 2009. Song J, Curtin WA. Acta Mater 2011;59:1557–69. Barnoush A, Vehoff H. Acta Mater 2010;58:5274–85. Martin ML, Fenske JA, Liu GS, Sofronis P, Robertson IM. Acta
Mater 2011;59:1601–6. Martin ML, Robertson IM, Sofronis P. Acta Mater 2011;59:3680–7. Hirth JP. Metall Trans A 1980;11:861–90. Troiano AR. Trans Am Soc Met 1960;52:54–80.
 Oriani RA. Corrosion 1987;43:390–7. Gerberich WW, Oriani RA, Lii M-J, Chen X, Foecke T. Philos Mag
A 1991;63:363–76. Birnbaum HK, Sofronis P. Mater Sci Eng, A 1994;176:191–202. Robertson IM, Lillig D, Ferreira PJ. In: Somerday BP, Sofronis P,
Jones R, editors. Hydrogen in metals. Jackson Hole (WY): ASMInternational; 2009.
 Nagumo M. ISIJ Int 2001;41:590–8. Nagumo M. Mater Sci Technol 2004;20:940–50. Gerberich WW, Stauffer DD, Sofronis P. In: Somerday BP, Sofronis
P, Jones R, editors. Effects of hydrogen on materials. Proceedings ofthe 2008 international hydrogen conference. Jackson Hole(WY): ASM International; 2009. p. 38–45.
 Sakaki K, Kawase T, Hirato M, Mizumo M, Araki H, Shirai Y, et al.Scripta Mater 2006;55:1031–4.
 Takai K, Shoda H, Suzuki H, Nagumo M. Acta Mater2008;56:5158–67.
 Srinivasan R, Neeraj T. Unpublished research. San Marchi C, Somerday BP, Nibur KA, Stalheim DG, Boggess T,
Jansto S. PVP2010. Bellevue (WA): ASME; 2010. p. 25825. San Marchi C, Somerday BP, Nibur KA, Stalheim DG, Boggess T,
Jansto S. PVP2011. Baltimore (MD): ASME; 2011. p. 57684. Hansen N, Juul Jensen D. Mater Sci Technol 2011;27:1229–40.
T. Neeraj et al. / Acta Materialia 60 (2012) 5160–5171 5171
 Hughes DA, Hansen N. Acta Mater 1997;45:3871–86. Wilsdorf HGF. Mater Sci Eng 1983;59:1–39. Li S, Li J, Neeraj T, Srinivasan R. Unpublished research. Hull D. Fractography: observing, measuring and interpreting fracture
surface topography. Cambridge: Cambridge University Press; 1999. Lyles Jr RLW. Acta Metall 1975;23:269–77. Wilsdorf HGF. Acta Metall 1982;30:1247–58. Cuitino AM, Ortiz M. Acta Mater 1996;44:427–36. Farrell K. Radiat Eff 1980;53:175–94. Zinkle SJ, Wolfer WG, Kulcinski GL, Seitzman LE. Philos Mag A
1987;55:127–40. Bringa EM, Traiviratana S, Meyers MA. Acta Mater
 Tang Y, Bringa EM, Remington BA, Meyers MA. Acta Mater2011;59:1354–72.
 Traiviratana S, Bringa EM, Benson DJ, Meyers MA. Acta Mater2008;56:3874–86.
 Zhu T, Li J. Prog Mater Sci 2010;55:710–57. Wang YZ, Li J. Acta Mater 2010;58:1212–35. Suresh S. Fatigue of materials. 2nd ed. Cambridge: Cambridge
University Press; 1998. Wu YC, Teng MK, Hsia Y, Chang XR, Tian ZZ, Hsiao CM. Mater
Sci Forum 1995;175–178:573–6. Desai SK, Neeraj T, Gordon PA. Acta Mater 2010;58:5363–9. Tateyama Y, Ohno T. Phys Rev B 2003;67:174105.